Featured at the proceedings FIB-symposium “Concrete and environment” in Berlin,October 2001Durability of Resource Saving “Green” Types of ConcreteM.Sc. Marianne Tange Jepsen, B.Sc. Dorthe Mathiesen,and Centre Manager, M.Sc. Christian Munch-PetersenConcrete Centre, Danish Technological InstituteTaastrup, DenmarkChief Concrete Technologist, Ph.D. Dirch BagerCement and Concrete Laboratory, Aalborg PortlandAalborg, DenmarkSummaryOne of the impediments for the use of resource saving "green" types of concrete on a largerscale is the lack of documentation of durability properties. The Danish Centre for ResourceSaving Concrete has carried out durability investigations to encourage the use of greenconcrete. This article presents the results of an investigation of frost resistance, carbonationand chloride ingress for five types of green concrete. The investigation shows that the testedtypes of green concrete can be evaluated using the same accept criteria as for ordinary typesof concrete. Some of the residual products lower the effect of the chemical additives, e.g. theair entraining agent, and therefore it can be difficult to obtain an air void structure withsufficient fineness to ensure frost resistance. However, it seems possible to produce greenconcrete, which is just as durable as ordinary concrete.IntroductionIn Denmark, a Centre for Resource Saving Concrete Structures was formed in 1998. The aimis to gain more knowledge about environment-friendly – so-called “green” - types of concreteand to develop technical solutions, so green concrete can be used in modern buildingtechnology. Fulfilment of the objectives of the centre calls for different kinds of expertise.Therefore, the centre involves partners from all sectors related to concrete production, i.e.cement and aggregate producers, a contractor, a ready mix plant, a consultant and a buildingowner besides Danish Technological Institute and the two technical universities in Denmark.The ways to sustainable concrete design are manifold. The Centre aims for• concrete with minimal clinker content• concrete with green types of cement and binders• concrete with inorganic residual products• operation and maintenance technology for green concrete structures• green structural solutions and structural solutions for green concreteThe centre has initiated five development projects corresponding to the five targets. The threefirst mentioned all imply changes of the traditional concrete mix design. Investigation ofdifferent concrete mix designs has been carried out in different phases: The first phaseconsisted of a screening of more than 30 different mix designs. Among these, the mostpromising mix designs were selected for a comprehensive test programme in the secondphase. The results presented in this article originate from this second phase, frominvestigations of the durability of five green types of concrete intended for use in aggressiveenvironment.In the year 2001 the practical use of green concrete and green structural solutions will bedemonstrated, when the results of the development projects are incorporated in a highwayoverpass project.1
Environmental goals and intentionsThe Centre for ressource saving concrete has laid down a list of environmental goals:• CO 2 emission caused by concrete production must be reduced by at least 30%.• The concrete must consist of at least 20% residual products, used at aggregates.• The concrete industry’s own residual products must be used in concrete production• New types of residual products, previously landfilled or disposed of in other ways, mustbe used in concrete production• CO 2 -neutral, waste-derived fuels must replace at least 10% of the fossil fuels in cementproduction.The Centre defines “green” concrete as concrete which satisfies one or more of theenvironmental goals. Moreover, a green type of concrete has to meet all of the environmentalintentions listed below:• avoid the use of materials which contain substances on the Danish EnvironmentalProtection Agency’s list of unwanted materials• do not reduce the recycling ability of green concrete compared to conventional concrete(today, 95% of the concrete is reused)• do not increase the content of hazardous substances in discharge water from concreteproductionThe environmental aspects of the project is described in greater detail in .Test programmeObjectivesDepending on the environmental action the concrete will be subjected to most concrete codesstate demands on e.g. maximum w/c ratio, minimum strength and minimum filler content (seefor example DS 481 ). We know by experience that these requirements will lead to denseand durable concrete structures. But how do we know that these requirements are sufficientfor types of concrete differing from conventional concrete, e.g. green types of concrete, wherewe have very limited experience? Therefore, in order to encourage the use of green types ofconcrete, one important task is to provide documentation of their durability properties and toprove that they have adequate service lives.A number of standard test methods have been developed to test concrete resistance againstspecific deterioration mechanisms, e.g. salt surface scaling and chloride ingress. When testingnew types of concrete using standard test procedures prepared for conventional concrete, onemay face two problems:• The test results approve non-durable concrete or disqualify durable concrete, because theaccept-criteria are not adjusted to the present type of concrete.• The standard tests do not uncover new durability problems introduced with new types ofconcrete, because the standard tests only relate to deterioration mechanisms relevant forconventional concrete.The chemical composition of the green constituents in the concretes in this study has beenthoroughly examined. In the light of this examination, it is believed that the concretes tabledin the next paragraph will not present any new durability aspects, so therefore thisinvestigation is focused on the classical durability issues of frost resistance, chloride ingress,and carbonation.The standard test procedures chosen areFrost resistance: Surface scaling according to a modified SS 13 72 44 (Borås method) ,and air void analysis according to DS/EN480-1 .
Carbonation: NT-BUILD 357 .Chloride ingress: CTH-method .All these methods prescribe testing of time dependent properties at fixed deadlines, e.g. 28days after casting. However, in the preliminary testing of green concretes it has been observedthat the development of strength for some of the green types of concrete deviate from strengthdevelopment of conventional concrete, and it is most likely that the development of otherproperties will deviate too. For this reason, measurements of surface scaling and chloridediffusion coefficient have been carried out at more than one concrete age.Concrete mix designsThe investigation includes five green types of concrete. In addition, a reference concrete, AR,is included in the test programme. AR is a normal Danish concrete intended for aggressiveenvironment. AR is produced with extra low alkali, highly sulphate resistant cement, amoderate fly ash content as well of a moderate content of silica fume. It fulfils the Danishcode DS 481  and the specification for concrete work of the Danish Road Directorate .The five green types of concretes are:A0 Concrete with low alkali, moderate sulphate resistant cement. Change of cement typelowers the energy consumption of cement production. The same cement type is usedfor A1 and A3. A0 fulfils DS481, but not the specification of the Danish RoadDirectorate.A1 Concrete with a high amount of fly ash (40% of powder b.w.)A3 Concrete with sewage sludge incineration ash instead of ordinary fly ashA5 Concrete with concrete slurryA6 Concrete with stone dustThe compressive strengths of the green types of concrete are all comparable to the strength ofAR. The concrete mix designs are listed in Table 1.Table 1: Mix design for the tested concretes (according to the batch report from the ready mixplant). All constitutents are noted by weight [kg/m 3 ].Constituent Description AR A0 A1 A3 A5 A6Cement Aalborg Portland 287.6 - - - - -LASR cement(CEM I 42.5 HS/EA)Aalborg PortlandRAPID ® cement (CEMI 52.5 MS/LA)- 286.5 188.6 277.0 - -Cementa- - - - 398.0 397.2ANL cement(CEM I 42.5 HS/LA)Ordinary Danaske B1 33.7 32.3 137.4 - - -fly ashSilica fume Elkem 17.4 17.0 17.8 17.0 - -Residual Fly ash/sewage plant - - - 34.7 - -product Concrete slurry(weight of dry matter)- - - - 14.6 -Stone dust 0/2 462Water 149.0 155.4 131.7 143.3 147.9 150.0Plastizicer Conplast 212 2.39 2.50 2.42 2.23 -Peramin V - - - - - 1.98SuperplastizicerConplast SP 605 - - 3.40 3.18 - -
Constituent Description AR A0 A1 A3 A5 A6Peramin F - - - - 3,95 -CEM 92M - - - - - 6.78Air-entraing Conplast 316 AEA 1:5 1.01 0.73 0.50 0.31 - -admixture HPa - - - - 0,12 0,15SandCoarseaggregate0/4 A, Nr. Haldne 621 629 646 640 - -0/8 Östervang 832 4574/8 A, Uddevalla 244 245 251 249 - -8/16 A, Uddevalla 855 858 871 865 - -8/16 Östervang 200 19716/25 Östervang 718 693AR, A0, A1, and A3 is produced by a Danish ready mix plant, whereas A5 and A6 is producedby a Swedish concrete producer.The above mentioned concretes present a mix of different ways to lower the environmentalimpact of concrete production. Substitution of cement with fly ash (A1) is the traditional wayto minimise the clinker content. A0, A1, and A3 are produced with a green type of cement,where 9% of the fuel for cement production comes from renewable resources. A3, A5, and A6introduce new residual products in concrete production, A5 and A6 from the concrete industryitself, A3 from other industries. An evaluation of the environmental goals is given in Table 2.Table 2: Evaluation of environmental goals.Environmental goal A0 A1 A3 A5 A6• CO 2 reduction 27% (✓ ) 52% ✓ 29% (✓ )• Residual products as✓aggregates• Residual products from✓ ✓the concrete industry• Residual products from✓other sources• Waste-derived fuels 9% (✓ ) 9% (✓ ) 9% (✓ )A0 is accepted as a green type of concrete; though it does not fulfil any of the goals, it is closeto fulfilling two of the five goals.Resistance against frost deteriorationResultsThe test method used is an accelerated frost-thaw test according to SS 13 72 44, except each7 th frost-thaw cycle is replaced by 24 hours at constant temperature (20°C), which enablesregistration of ultrasound transmission time and dilation of the test specimens .The measurements of scaling are shown in Figure 1.
10001000scaling [g/m2]800600400200ARA0A1A3A5A6scaling [g/m2]800600400200ARA0A1A3A5A600 7 14 21 28 35 42 49 56time [days]00 7 14 21 28 35 42 49 56time [days]Figure 1: Results of surface scaling test according to SS 13 72 44 (modified). Left:Exposureto frost-thaw cycles started 31 days after casting (standard procedure). Right:Exposure to frost-thaw cycles started 59 days after casting.The concretes were also subjected to an air void analysis according to DS/EN480-1, see Table1.Table 3: Results of air void analysisAR A0 A1 A3 A5 A6Air content in hardened concrete [vol-%] 6.18 5.86 5.23 6.44 4.04 3.94Paste content [vol-%] 26.1 27.0 26.3 25.6 28.2 27.1Powers spacing factor [mm] 0.13 0.18 0.33 0.30 0.17 0.35Volume of micro air voids(diameter < 300 µm)[vol-%] 3.00 2.25 0.84 0.83 2.03 0.72CommentsNormally the salt scaling test is performed in a way that the exposure to frost-thaw cyclesstarts 31 days after casting. In this case, the accept criterion according to DS481 is that at leastone of the following two requirements has to be fulfilled:• The scaling after 56 freeze-thaw cycles is less than 0.2 kg/m 2• The scaling after 56 freeze-thaw cycles is less than 0.5 kg/m 2 and the proportion betweenthe amount scaled of after 56 cycles and the amount scaled of after 28 cycles is less than2.As can be seen in Figure 1, all concretes except A1 (concrete with high fly ash content) can beaccepted.A1 probably fails due to the high spacing factor. According to the Danish concrete code, thespacing factor of a concrete, which is not subjected to a frost-thaw test, must not exceed 0.20mm. If A1 had fulfilled this requirement, it would probably also show sufficient frostresistance. A review of relevant litterature shows that it is possible to make frost resistantconcrete with high fly ash contents if the fineness of the air void system is adequate (see e.g.).A6 has an even higher spacing factor than A1, though nearly no scaling was observed. At firstsight this seems contradictory, but observations made by Pigeon can explain this : Pigeonshowed that the critical spacing factor is not a fixed quantity valid for all types of concrete.The critical spacing factor is lower, the denser the concrete is. In addition to fly ash, A1 alsocontains silica fume, and A1 is expected to be denser than A6 without silica fume. For thisreason the critical spacing factor of A1 may be lower than 0.33, whereas the critical spacingfactor of A6 is higher than 0.35.
Effect of age of concrete, when the scaling test is performedAccording to the standardised test procedure of the scaling test, the concrete is exposed tofrost action for the first time 31 days after casting. In this study, a similar test has been run,where the age of the test specimens was 59 days, before they were exposed to frost. Theresults are shown in Figure 1 (to the right).A comparison of results shows that the scaling of A1 is reduced, when the concrete age isincreased before frost action. However, the scaling of A1 is still not satisfactory.For A3 a slight increase of scaling is observed at the later age. For the rest of the concretes,the amount of scaling is more or less unchanged. For all concretes except A1 it is difficult todraw conclusions about the time dependent development of frost resistance, because it is notpossible to detect a significant change, when the scaling in both tests were low.Inner damageParallel to the scaling test, the test specimens were inspected by measuring ultra soundtransmission time and dilation to reveal if any inner damage had occurred. However, thechanges in ultrasound transmission time and the length changes were small, so there is no signof inner deterioration.CarbonationMethod35 days after casting, the test specimens are placed in a climate chamber with a CO 2 enrichedatmosphere (3% CO 2 , 60% RH). The carbonation depth is measured 4, 8, and 12 weeks afterthe specimens have been placed in the chamber (the carbonation depth is made visible bymeans of phenolphthalein, according to NT-BUILD 357).ResultsThe results (mean values of carbonation depth) are shown in Figure 2.20carbonation depth [mm]1510504 8 12time [weeks]ARA0A1A3A5A6Figure 2: Carbonation depths measured according to NT-BUILD 357.CommentsThe carbonation depths of A0 and A3 are at about the same level as the carbonation depth ofthe reference concrete AR. The carbonation is more pronounced for A1 and less pronouncedfor A5 and A6.Calcium hydroxide, Ca(OH) 2 , is formed during cement hydration, and because of the highalkalinity of calcium hydroxide, the presence of calcium hydroxide will ensure a high pH-
value in the concrete. The pH-value is roughly constant, as long as calcium hydroxide ispresent, no matter the content of calcium hydroxide.During the carbonation process, calcium hydroxide reacts with carbon dioxide, CO 2 , from theatmosphere. When all calcium hydroxide in an area has reacted, the pH-value in the areadecreases. If two types of concrete have different initial contents of calcium hydroxide, theone with the lowest content will be most sensitive to carbonation, because the carbonationfront will travel faster. That means that the initial content of calcium hydroxide in hardenedconcrete expresses a kind of carbonation potential.The initial content of calcium hydroxide has been calculated for the six types of concrete inthis study by calculating the amount of calcium hydroxide formed during cement hydrationand correcting the result by the amount of calcium hydroxide consumed during a pouzzolanicreaction with fly ash or silica fume. The calculation shows that the initial content of calciumhydroxide is about the same for AR, A0, and A3 (~30 kg/m 3 concrete). The amount of fly ashin A1 is so high that it can eliminate all the calcium hydroxide. For A5 and A6 the initialcontent of calcium hydroxide is higher than that of the reference AR (~110 kg/m 3 ). Theseresults indicate that A1 will be more sensitive to carbonation than AR, A0, and A3, whereas A5and A6 will be far less sensitive. This agrees very well with the experimental findings, thoughin A1 there is still an amount of calcium hydroxide left after the puzzolanic reaction, whichcan be observed because there is still an area with high pH-value in front of the carbonatedarea.It is important to notice that the difference in carbonation potential between AR and A5 andA6 does not come from the green elements in A5 and A6 (concrete slurry and stone dust,respectively). According to the explanation given above, the difference is due to differences inDanish and Swedish concrete practice: Swedish concrete has a higher cement content andcontains no puzzolans, and therefore it will in general be more resistant to carbonation thanDanish concrete.Chloride ingressTest MethodFor this part of the project, a rapid chloride migration test method was used . The method,which is developed at Chalmers University of Technology, is known as the CTH-method, butit is also an Nordtest standard (NT-BUILD 492). This test method was considered the mostadvantageous for the purpose in this project for the following reasons:• Most other rapid test methods (i.e. AASHTO T277) measure the charge passing thespecimen when a voltage is applied over it. The charge is very dependent on the ioncontent in the pore solution, not only the chloride ions. The ion composition in the poresolution may vary a lot from one green type of concrete to another, because of e.g. theresidual products used, and therefore a comparison of results would be difficult. Using theCTH-method, the chloride diffusion coefficient is evaluated from a measurement ofchloride penetration depth. That is, the result is based on a direct measurement of chlorideions present in the sample.• Ponding tests (e.g. NT-BUILD 443) register the chloride profile after exposure to a saltsolution. The test period is often several months, which means that the registeredresistance against chloride ingress is a kind of average resistance during the test period. Incontrast, the test period of the CTH-method is limited to some hours, which enablesmeasurement of the resistance against chloride ingress at a certain age.• In general, the CTH-method is theoretically clear, experimentally simple, and it hasshown good repeatability.ResultsFor each type of concrete, the chloride diffusion coefficient is measured 28 days, 3 monthsand 1 year after casting. The measured chloride diffusion coefficients are shown in Figure 3.
eason for the differences is the general differences between Danish and Swedish concretetradition, where concrete in Sweden is produced without fly ash and silica fume.Accept criterionIn the Danish and Swedish concrete codes, no acceptance criteria are stated for the chloridediffusion coefficient. Tang Luping has given the following guidelines for the chloridediffusion coefficient D measured with the CTH-method 28 days after casting:• D
References DAMTOFT, J.S., GLAVIND, M., and MUNCH-PETERSEN, C., “Danish Centre forGreen Concrete”, accepted for publication in proceedings from CANMET/ACIInternational Symposium on Sustainable Development of Cement and Concrete, SanFransisco, September 2001. DS 481, “Concrete - Materials”, 1 st ed. (in Danish: “Beton – Materialer”), DanishStandards Association, Copenhagen, 1999. LUPING, T., “Modified Slab Test. Test Method for the Freeze-Thaw resistance ofConcrete – Scaling and Cracking”, SP, Borås, 1999. DS/EN 480-1, “Admixtures for concrete, motar and grout – Test methods – Part 11:Determination of air void characteristics in hardened concrete”, Danish StandardsAssociation, Copenhagen, 1999. NT-BUILD 357, “Concrete, repairing materials and protective coating: Carbonationresistance”, NORDTEST, Espoo, 1989. “Evaluation of the Rapid Test Method for Measuring the Chloride DiffusionCoefficients of Concrete. Appendix 1: The CTH Rapid Test, version used in roundrobin test of the Nordtest project No. 1388-98”, SP Rapport 1998:42, SP, Borås, 1998. “Directions for construction of concrete bridges” (in Danish: “Udbuds- oganlægsforskrifter. Betonbroer. Almindelig arbejdsbeskrivelse), Danish Road directorate,Copenhagen, 2000. MALHOTRA, V. M., and RAMEZANIANPOUR, A. A., “Fly ash in concrete”, 2 nd ed.,CANMET, Ottawa, 1994. PIGEON, M., “La durabilité au gel du béton”, Materials and Structures, Vol. 22, No.127, pp. 3-14. TANG, L., and NILSSON, L.-O., “Chloride diffusivity in high strength concrete atdifferent ages”, Nordic Concrete Research, Publication No. 11, pp. 162-171.